The γ-phase of SrTeO~3~ at 583K
Zavodnik, Valery E.; Ivanov, Sergey A.; Stash, Adam I.; Acta Crystallographica Section E 63 (2007) i151–i151; doi:10.1107/S1600536807026098

data_2214074
_publ_section_title
;
 The \g-phase of SrTeO~3~ at 583K
;
_journal_coeditor_code           BR2042
_journal_issue                   7
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i151
_journal_page_last               i151
_journal_paper_doi               10.1107/S1600536807026098
_journal_volume                  63
_journal_year                    2007
_chemical_formula_iupac          'Sr Te O3'
_chemical_formula_moiety         'O3 Te, Sr'
_chemical_formula_structural     'Sr Te O3'
_chemical_formula_sum            'O3 Sr Te'
_chemical_formula_weight         263.22
_chemical_name_systematic
;
strontium tellurite
;
_space_group_IT_number           5
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 122.21(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            24
_cell_length_a                   28.262(6)
_cell_length_b                   5.9350(10)
_cell_length_c                   15.434(3)
_cell_measurement_reflns_used    24
_cell_measurement_temperature    583(2)
_cell_measurement_theta_max      14.5
_cell_measurement_theta_min      12.3
_cell_volume                     2190.4(10)
_computing_cell_refinement       CAD-4-PC
_computing_data_collection       'CAD-4-PC (Enraf--Nonius, 1993)'
_computing_data_reduction        CAD-4-PC
_computing_molecular_graphics    'DIAMOND (Brandenburg, 2005)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      583(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type
'Enraf--Nonius CAD-4 with high-temperature device'
_diffrn_measurement_method       \w/2\q
_diffrn_radiation_monochromator  \b-filter
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           AgK\a
_diffrn_radiation_wavelength     0.56086
_diffrn_reflns_av_R_equivalents  0.0786
_diffrn_reflns_av_sigmaI/netI    0.1609
_diffrn_reflns_limit_h_max       34
_diffrn_reflns_limit_h_min       -30
_diffrn_reflns_limit_k_max       0
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            2335
_diffrn_reflns_theta_full        19.97
_diffrn_reflns_theta_max         19.97
_diffrn_reflns_theta_min         2.08
_diffrn_standards_decay_%        0
_diffrn_standards_interval_time  60
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    12.0360
_exptl_absorpt_correction_T_max  0.3887
_exptl_absorpt_correction_T_min  0.1408
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(Alcock, 1970)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    4.789
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             2736
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.09
_refine_diff_density_max         2.514
_refine_diff_density_min         -2.180
_refine_ls_extinction_coef       0.00036(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL97
_refine_ls_goodness_of_fit_ref   0.935
_refine_ls_matrix_type           full
_refine_ls_number_parameters     183
_refine_ls_number_reflns         2285
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      0.934
_refine_ls_R_factor_all          0.1120
_refine_ls_R_factor_gt           0.0423
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     'calc w=1/[\s^2^(Fo^2^)+(0.0585P)^2^]'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0957
_refine_ls_wR_factor_ref         0.1029
_reflns_number_gt                1156
_reflns_number_total             2285
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            br2042.cif
_cod_data_source_block           I
_cod_original_cell_volume        2190.4(8)
_cod_original_sg_symbol_H-M      'C 2'
_cod_database_code               2214074
_cod_database_fobs_code          2214074